Effect of the ionic product of bioglass 60s on osteoblastic activity in canines
- 955 Downloads
The objective of the present study was to evaluate the effect of the ionic product (IP) of BG60S on osteoblastic activity. The following media groups were created: DMEM, which is formed by osteoblasts in basal medium; IP DMEM, which is formed by osteoblasts in IP with basal medium; OST, which is formed by osteoblasts in osteogenic medium; and IP OST, which is formed by osteoblasts in IP with osteogenic medium. The osteoblasts were cultivated in an incubator at 37 °C and 5 % CO2 for 7, 14 and 21 days. After each period, the alkaline phosphatase (AP) activity, mineralised area per field and expression of osterix (OSX), bone sialoprotein (BSP), osteonectin (ON) and osteocalcin (OC) were evaluated by reverse transcription (RT)-PCR.
The IP significantly increased the AP activity in the IP DMEM group at 7 and 14 days and reduced the AP activity in the IP OST group at 14 and 21 days relative to their respective controls (DMEM and OST). The groups that received the IP displayed a significant increase in the percentage of mineralised area per field and more advance maturation of the extracellular matrix relative to those that did not receive IP. The IP significantly increased the expression of OSX, BSP and ON in osteoblast cultures maintained in IP DMEM compared with the control (DMEM) for the majority of studied periods. In osteogenic medium, IP also significantly increased OSX, BSP, ON and OC expression compared with the control (OST) for the majority of studied periods.
The IP of BG60S alters the gene expression of canine osteoblasts, favouring the synthesis and mineralisation of the extracellular matrix.
KeywordsOrthopaedics Biomaterials Bone substitute Osteoblasts
Analysis of variance
Bone morphogenetic protein-2
Animal experimentation ethics committee (Comitê de Ética em Experimentação Animal)
Dulbecco’s modified Eagle’s medium (basal medium)
Foetal bovine serum
Nitroblue tetrazolium salt
Centre for Stem Cells and Animal Cell Therapy (Núcleo de Células Tronco e Terapia Celular Animal)
- IP DMEM
Ionic product in basal medium
- IP OST
Ionic product in osteogenic medium
Penicillin, streptomycin and amphotericin
Quantitative reverse transcription polymerase chain reaction
Runt-related transcription factor 2
Sodium dodecyl sulphate
Federal University of Minas Gerais (Universidade Federal de Minas Gerais)
University of Uberaba (Universidade de Uberaba)
Wingless-type MMTV integration site family
Bioglass 60S (BG60S) has a molar composition of 4 % P2O5, 36 % CaO and 60 % SiO2, is a biomaterial with favourable characteristics for bone regeneration  and displays beneficial effects on the repair of bone defects in dog jaws . But nothing is known about the effect of this biomaterial on the activity of dog osteoblasts, especially as regards the production of extracellular matrix and osteogenic differentiation. Generally speaking, when the bioglass is implanted on the bone tissue, it provides a framework for migration and colonization by osteoblasts, and apart from this, it reacts with the interstitial fluids, releasing ions, mainly calcium and silicon , which are, probably, primarily responsible for the biological effect.. These ions may favour osteogenic proliferation [4, 5] and differentiation in vitro [5, 6]. However, the ideal chemical composition of bioglass that releases the ideal combination and concentration of ions to maximise the bone regeneration process upon implantation is not well understood. In an in vitro study with rat osteoblasts, BG60S exhibited satisfactory Ca and Si release rates, which favours cellular proliferation . However, the effects of this biomaterial on canine osteoblast activity are unknown. Osteoblasts perform a crucial function in the bone regeneration process by producing and secreting the extracellular bone matrix. The objective of the present study was to investigate the hypothesis that the ionic product (IP) of BG60S will increase the synthesis and mineralisation of the extracellular matrix by evaluating the effect of the IP on canine osteoblastic activity.
Concentrations of Si and Ca ions in cell culture media
When added to cell culture media, BG60S was partially dissolved, causing a significant increase in the concentration of Si and Ca ions. The concentration of Si ions was 40.91 mg/L in IP DMEM medium (which is formed by osteoblasts in IP with basal medium), 41.28 mg/L in IP OST medium (which is formed by osteoblasts in IP with osteogenic medium) and lower than 1 mg/L in the media with no contact with BG60S (DMEM and OST, which are formed by osteoblasts in basal medium and osteoblasts in osteogenic medium, respectively). The concentration of Ca ions was 96.5 mg/L in DMEM medium, 87.5 mg/L in OST medium, 169 mg/L in IP DMEM medium and 156.5 mg/L in IP OST medium. Hence, BG60S increased the concentration of Ca ions by 75 and 79 % in basal and osteogenic media, respectively.
Alkaline phosphatase activity
Evaluation of the mineralised matrix synthesis
Quantification of gene transcriptions for OSX, BSP, ON and OC
The biological effect of biomaterials can be evaluated by their dissolution product  because the ions liberated during dissolution contribute for the biological effect . The increased concentration of Si (more than 400 %) and Ca ions (more than 75 %) from the dissolution of BG60S was expected; however, it was significantly higher than the values reported in the literature with bioglass of different compositions [8, 9]. This result indicates that the same type of biomaterial can produce different results according to the specific composition, which explains the various responses found in the literature.
The increase in AP activity in group IP DMEM relative to group DMEM at 7 and 14 days suggests a stimulating effect of the IP on the secreting activity of the osteoblast. AP is an enzyme that occurs in the membrane of the osteoblast, and it directly participates in the synthesis and mineralisation of bone matrix . This enzyme is commonly used as a marker of osteogenic differentiation  and a parameter for the evaluation of the bone activity, and high AP activity also indicates high osteoblastic activity .
The significant increase of the extracellular matrix area and greater mineralisation of the extracellular matrix observed in cultures that received the IP shows the stimulating effect that IPs of BG60S have on osteoblasts with regard to matrix synthesis and mineralisation. The synthesis and mineralisation of the extracellular matrix are considered the most reliable and representative parameters of in vitro osteoblastic activity . The predominant increase of OSX, BSP and ON expression in the cultures that received the IP relative to those that did not suggests that the IP of BG60S stimulates the synthesis and mineralisation of the extracellular matrix by increasing the expression of these proteins. OSX is a specific transcription factor of osteogenic differentiation [13, 14] that acts on the transformation of pre-osteoblasts into mature osteoblasts [10, 15]. Furthermore, OSX acts on the synthesis and mineralisation of bone matrix via the intranuclear receptor of vitamin D and on the inhibition of osteoblastic proliferation via the inhibition of Wnt (Wingless-type MMTV integration site family) signalling [13, 14]. BSP and ON are non-collagen proteins in bone matrix used as markers of osteogenic differentiation and osteoblastic activity [11, 16, 17]. These proteins are intimately related to the synthesis and mineralisation process of extracellular bone matrix . Although the IP did not clearly increase OC expression, the increase in its expression in the IP OST group at 14 and 21 days suggests that the ions released by BG60S can also positively influence its expression. OC is a specific bone tissue glycoprotein expressed by osteoblasts and is considered the main non-collagen protein of bone matrix [16, 17]. The evaluation of its expression can be used for monitoring bone metabolism .
The beneficial effects of the IP of BG60S on osteoblastic activity are most likely caused by the Si and Ca ions released during its dissolution process. Studies with rat osteoblast cultures have demonstrated that Si can increase cellular activity and proliferation  as well as the expression of runx2, collagen type 1 and ON . Furthermore, Si can favour the mineralisation of extracellular matrix . Ca is another ion released during BG60S dissolution, and it can increase the activity and proliferation of human mesenchymal stem cells [4, 5]. Studies have indicated that extracellular Ca can increase osteopontin, OC, BSP and bone morphogenetic protein-2 (BMP 2) expression in human mesenchymal stem cells . Additionally, Ca favours the synthesis and mineralisation of extracellular matrix by human mesenchymal stem cells . The previously mentioned studies have indicated that Ca favours in vitro osteogenesis; however, little is known of the mechanisms involved. The increase in extracellular Ca can increase the expression of osteopontin and BSP in mouse pre-osteoblasts, an effect mediated by L-type Ca channels and the Ca/calmodulin-dependent protein kinase 2 (CaM-CaMK2) signalling pathway .
With the limitations of the current study, there is only assessment of the 60S bio-glass in the form of its ionic product. Although assessment of the product of dissolving the 60S bio-glass may bring important information concerning its form of action, the biological response of a biomaterial may also be influenced by the size, form, microstructure, texture and topography of the implant surface. Thus, it is important to carry out complementary studies that may assess all these variables, allowing for a better understanding as to how each one of them influences its biological response.
The IP of BG60S alters the gene expression of canine osteoblasts, favouring the synthesis and mineralisation of extracellular matrix.
This study was performed according to the international norms for animal welfare and approved by the UFMG Animal Experimentation Ethics Committee (protocol n. 157/2009).
Biomaterial and ionic product
BG60S with a molar composition 4 % P2O5 36 % CaO 60 % SiO2 was produced with 133.8 mL tetraethyl orthosilicate (TEOS), 13.6 mL triethyl phosphate (TEP), 97.9 mL deionised water, 16.3 mL 2 N nitric acid solution and 85.01 g Ca nitrate [Ca(NO3)2 4H2O] in accordance with the protocol described by Coelho et al. . The biomaterial was incubated at 60 °C for 72 h for gelation and maturation and then remained at 60 °C for 72 h for drying, which was followed by gradual temperature increase of 10 °C every 24 h until reaching 120 °C. After drying, the sample was milled, and the grain size fraction smaller than 137 μm was separated. The elimination of possible residues was performed by heating in a muffle furnace at 700 °C for 6 h and applying a heating and cooling rate of 1 °C per minute. To obtain the IP, 6 g biomaterial was added to 1 L low-glucose Dulbecco’s modified Eagle’s medium (Gibco, CA, USA) containing gentamicin (60 μg/L), penicillin (100 U/mL), streptomycin (100 μg/mL) and amphotericin (25 μg/mL) (PSA, Sigma-Aldrich, USA). The mixture was homogenised and incubated for 12 h at 6 °C. After incubation, the suspension was filtered using a 22 μm membrane, and the pH was adjusted to 7.2, which resulted in the IP of BG60S.
Concentrations of Si and Ca ions in the cell culture media
Prior to the use of the culture media with canine osteoblasts, the concentration of Si and Ca ions in the media was measured. The atomic absorption spectrometry technique (GBC-Avanta) was used according to the standard addition method to determine the ion concentration.
Preparation and cultivation of osteoblasts and formation of the experimental groups
A canine osteoblast culture (CnOb - canine osteoblasts, Cell Application, CA, USA) was used to evaluate the effect of the IP of BG60S. The culture was defrosted, and then the pellet was plated and cultivated in T75 flaks with low-glucose DMEM (Gibco, CA, USA) containing gentamicin (60 μg/L), penicillin (100 U/mL), streptomycin (100 μg/mL) and amphotericin (25 μg/mL) (PSA, Sigma-Aldrich, USA) and enriched with 10 % foetal bovine serum (FBS - Soralis, Brazil) [basal medium]. The flasks were maintained in an incubator at 37 °C and 5 % CO2. The culture medium was changed twice per week, and when 80–90 % confluence was achieved, the cells were subcultured. On the third subculture after obtaining 80–90 % confluence, the osteoblasts were used for the evaluation of the IP, and the following groups were formed: DMEM, IP DMEM [IP enriched with 10 % FBS], OST [basal medium enriched with ascorbic acid (50 μg/mL), ß-glycerophosphate (10 mM) (Sigma-Aldrich, USA), dexamethasone (0.1 μM) (Aché, Brazil) and 10 % FBS] and IP OST [IP enriched with ascorbic acid (50 μg/mL), ß-glycerophosphate (10 mM), dexamethasone (0.1 μM) and 10 % FBS].
The osteoblasts were cultivated in quadruplicate at 37 °C and 5 % CO2 for 7, 14 and 21 days with DMEM, IP DMEM, OST or IP OST. Subsequently, the AP activity, mineralised area per field and the relative expression of OSX, BSP, ON and OC were evaluated in each group by reverse transcriptase (RT)-PCR.
Alkaline phosphatase activity
For the evaluation of AP activity, the osteoblasts of each group were cultivated separately in 24-well plates. At the end of each period, the cultures were washed with phosphate buffered saline (PBS - 0.15 molar). To each well, 200 μL of 5-Bromo-4-Chloro-3-Indolyl phosphate/nitroblue tetrazolium salt (BCIT/NBT) solution (Zymed Laboratories, USA) was added. The samples were incubated for 2 h in an oven at 37 °C and 5 % CO2 and observed under an optical microscope before the addition of 200 μL of sodium dodecyl sulphate (SDS)-10 % HCl. These samples were placed in an oven overnight at 37 °C and 5 % CO2, and then 100 μL from each well was transferred to 96-well plates and read by a spectrophotometer at 595 nm .
Evaluation of mineralised matrix synthesis
To evaluate the percentage of mineralised matrix per field, the osteoblasts of each group were cultivated separately in 6-well plates with cover slips (Sarstedt, USA). After each evaluation period, the osteoblasts were fixed with 70 % ethanol for 24 h and dyed using the Von Kossa method. The percentage of mineralised matrix per field was determined with an ocular micrometer containing a 121-point grid, with 25 fields and a 4× objective .
Quantification of gene transcription for OSX, BSP, ON and OC
Genes and nucleotide sequence of primers used for RT-PCR
Annealing temperature (°C)
Reference or Accession No.
(5′ to 3′ nucleotide sequences)
Neupane et al. 
Vieira et al. 
Neupane et al. 
Vieira et al. 
An analysis of variance (ANOVA) was performed, and the mean and standard deviation were determined for each variable. The means were compared by Student’s t-test using the program Graphpad Instat 3 (GraphPad Software Inc., USA). Differences were considered significant at P < 0.05.
The authors would like to thank the Foundation for Research Support of the State of Minas Gerais (Fundação de Amparo à Pesquisa do Estado de Minas Gerais – FAPEMIG) for funding the study, National Council of Scientific and Technological Research (Conselho Nacional de Desenvolvimento Científico e Tecnológico - CNPq) for the doctoral grant, and the Veterinary School, Laboratory of Molecular Biology of the Department of Immunology and Biochemistry of the Institute of Biological Sciences, Laboratory of Biomaterials of the Department of Metallurgical Engineering and Materials and Dean of the Research Office of the Federal University of Minas Gerais (Pro-Reitoria de Pesquisa da Universidade Federal de Minas Gerais) for the support required to conduct this study.
- 12.Bruedigan C, Driel MV, Koedam M, Peppel JV, van der Eerden BC, Eijken M, et al. Basic techniques in human mesenchymal stem cell cultures: differentiation into osteogenic and adipogenic lineages, genetic perturbations, and phenotypic analyses. Curr Protoc Stem Cell Biol. 2011;17:1–19.Google Scholar